Reactive and Functional Polymers 123 (2018) 61–69
Contents lists available at ScienceDirect
Reactive and Functional Polymers journal homepage: www.elsevier.com/locate/react
Complexation with whey protein hydrolysate improves cacao pods husk pectin surface active and emulsifying properties
Daniel Trujillo-Ramíreza, Consuelo Lobato-Callerosb, Angélica Román-Guerreroa, ⁎ Landy Hernández-Rodríguezb, Jose Alvarez-Ramirezc, Eduardo J. Vernon-Carterc, a
Departamento de Biotecnología, Universidad Autónoma Metropolitana-Iztapalapa, San Rafael Atlixco No. 186, Col. Vicentina, Ciudad de México C.P. 09340, Mexico Departamento de Preparatoria Agrícola, Universidad Autónoma Chapingo, Km 38.5 Carr. México-Texcoco, Texcoco, Estado de México C.P. 56230, Mexico c Departamento de Ingeniería de Procesos e Hidráulica, Universidad Autónoma Metropolitana-Iztapalapa, San Rafael Atlixco No. 186, Col. Vicentina, Ciudad de México C. P. 09340, Mexico b
A R T I C L E I N F O
A B S T R A C T
Keywords: Cacao pod husks pectin Whey protein hydrolysate Soluble complex Adsorption dynamics Emulsion stability
Pectin was extracted from cacao pod husks (CPHP) wastes, having a methylesteriﬁcation degree of 83.22%, acetylation degree of 10.20%, and protein content of 3.68%. The adsorption dynamics of CPHP at the canola oilwater interface were studied, and diﬀusion (kdiﬀ), penetration (kpen) and rearrangement (krea) rate constants were determined. Canola oil-in-water (O/W) emulsions (ECPHP) were stabilized which CPHP, and exhibited an initial area-volume mean diameter (d3,2) of 113.60 nm, which increased to 162.0 nm during 28 days of storage. CPHP was electrostatically complexed with whey protein hydrolysate (WPH) in a weight ratio 5:1 and pH 3.25, in order to improve the surface active and emulsifying activities. The soluble complex (SCWPH-CPHP) decreased the interfacial tension faster and to a lower value, and displayed higher kdiﬀ and kpen than CPHP. SCWPH-CPHP yielded O/W emulsions with d3,2 < 90 nm, which did not suﬀer signiﬁcant changes in oil droplet size during storage. The apparent viscosity of SCWPH-CPHP aqueous dispersion was much lower than that of CPHP dispersion. The zeta potential of EWPH-CPHP was lower than for ECPHP. Thus, it was concluded that the greater stability of EWPH-CPHP was due mainly to steric repulsion originated by the soluble complex adsorption layers around the oil droplets.
1. Introduction Pectin is a heteropolysaccharide exhibiting a wide diversity in its molecular structure. Basically it is a group of polysaccharides rich in galacturonic acid comprising homogalacturonan (HG; homopolymer mainly composed of ~65% of α-D-galactopyranosyluronic acid units), rhamnogalacturonan-I (RG-I, heteropolymer of units repeating α-Lrhamnosyl) and rhamnogalacturonan-II (branched pectic domain containing a HG backbone). The galacturonic acid residues may be partially methyl-esteriﬁed on the carboxyl group at C-6 position and Oacetylated at C-2 or C-3 depending on plant species [1–3]. The molecular weight of pectin (Mw), viscosity, the protein content, the degree of acetylation (DAc), amidation (DAmd) and methylesteriﬁcation (DM) are the main factors which dictate the functional properties of pectin [4,5]. Up to the last decade, most pectin applications stemmed from its gel-forming ability, rendering it as suitable to use as gelling, thickening, or stabilizing agent in a wide number of industrial domains, including the food, pharmaceutical and chemistry industries [6–8]. Nowadays,
this hydrocolloid is gradually gaining acceptance as an eﬀective emulsiﬁer and the emulsifying properties are being increasingly assessed in numerous industrial applications . Some pectins from different botanical sources have been tagged as showing surface-activity and to be capable of forming ﬁne oil droplets, including citrus peel pectin [10–12], sugar beet pectin [10,13–15], and hawthorn pectin . However, new sources of pectin from regional botanical sources and agroindustrial wastes continue to be explored. The cacao (Theobroma cacao L.) fruit is an important crop of several tropical and sub-tropical countries, and cacao beans are the main ingredient of the multi-billion worldwide chocolate industry. After the beans extraction, the pod husks (accounting for approx. 52–76% of the weight of the cacao fruit) are discarded and represent a serious environmental problem . Bazarte et al.  reported that for each ton of dry cacao beans, 10 tons of wet pod cacao husks were generated. The production of dry cacao beans for the period 2015/2016 was estimated as 3660 metric tons (36,600 metric tons of wet cacao pod husks) . Recently, Yapo and Koﬃ  reported that cacao pod husks pectin exhibited emulsifying activity and emulsion-stabilizing activity,
Corresponding author. E-mail address: [email protected]
https://doi.org/10.1016/j.reactfunctpolym.2017.12.011 Received 28 June 2017; Received in revised form 29 November 2017; Accepted 18 December 2017 Available online 19 December 2017 1381-5148/ © 2017 Elsevier B.V. All rights reserved.
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
pectin was ground in a mortar in order to obtain a ﬁne powder. Extraction yield was estimated as (1):
without providing information regarding the initial droplet size and the variation in droplet size of the oil-in-water emulsions with storage time. Pectin is a multifunctional ingredient susceptible to chemical and enzymatic conversions, and selective alterations of pectin molecular structure may render the polymer suitable for numerous applications. In this context the complexation between protein and polysaccharide molecules under special conditions of pH and weight ratio between both biopolymers can promote the formation of soluble complexes (SC), which may exhibit improved emulsifying properties than the individual biopolymers [21–24]. Thus, an ongoing research topic is the identiﬁcation and characterization of natural emulsiﬁers which have the potential of emulsifying and stabilizing emulsion oil droplets [25,26] and that can also be successfully used in food matrices [27–29]. Therefore, the objectives of this research were to: (a) obtain and characterize the pectin extracted from cacao pod husks (CPHP); (b) establish the conditions for obtaining whey protein hydrolysate (WPH)-CPHP soluble complex (SCWPH-CPHP); (c) evaluate the dynamic interfacial adsorption of SCWPH-CPHP, and (d) and to evaluate the stability of oil-in-water emulsions emulsiﬁed with SCWPH-CPHP in comparison to CPHP.
Yield (%) = (pectin powder (g)/cacao pod husk flour (g)) × 100%
Moisture content of CPHP was determined with a moisture analyzer (Ohaus, MB23, Parsippany, NJ, USA) by drying the sample at 105 °C to constant weight . 2.3. Physicochemical characterization of CPHP 2.3.1. Determination of the degree of methylesteriﬁcation (DM), degree of amidation (DAmd) and degree of acetylation (DAc) Degree of methylesteriﬁcation (DM), degree of amidation (DAm) and degree of acetylation (DAc) of CPHP was determined as reported by , with slight modiﬁcations. Pectin solution (0.500 g/100 mL of deionized water) was titrated with 0.1 mol/L NaOH using phenolphthalein as the indicator and the volume consumed was recorded as V1. Afterwards, saponiﬁcation of pectin was initiated by adding of 20 mL of 0.5 mol/L NaOH and allowed to react for 15 min under constant stirring. The reaction was stopped with the addition of 20 mL of 0.5 mol/L HCl. The excess HCl was neutralized by titration with 0.1 mol/L NaOH and the volume consumed was recorded as V2. Subsequently, the solution was saturated with 20 mL of 2.5 mol/L NaOH and mixed in a 1000 mL distillation ﬂask and connected to a condenser, whose delivery line was submerged into the mixture of 150 mL of deionized water and 20 mL of 0.1 mol/L HCl. The mixture was distilled until ~100 mL of the distillate was collected. The excess HCl was then titrated with 0.1 mol/L NaOH using methyl red as the indicator and the consumed volume was recorded as S. A blank test was performed using 20 mL of 0.1 mol/L HCl and the volume consumed of HCl was recorded as B. The diﬀerence of B and S was assumed to be V3. For determining the amount of acetyl, 0.500 g of the CPHP were dispersed in 25 mL of 0.125 mol/L NaOH, after stirring for 4 h, the solution was diluted in a 50 mL volumetric ﬂask to volume. An aliquot of 20 mL of diluted solution and 20 mL of Clark's solution (containing 100 g MgSO4·7H2O, 0.8 mL H2SO4 and 180 mL H2O) was transferred to a 1000 mL distillation ﬂask and the ﬁrst 15 mL of the distillate were collected by separated in a graduated cylinder. Immediately the steam supply was started and the distillation was continued until 150 mL of the distillate was obtained. This distillate was titrated with 0.05 mol/L NaOH to a pH of 8.5, and the volume required, in mL, was recorded as A. Deionized water was used as a blank for titration and the volume consumed was recorded as A0. The diﬀerence of A and A0 was assumed to be V4. Eqs. (2)–(4) were used for estimating DM%, DAmd% and DAc %:
2. Materials and methods 2.1. Materials Cacao fruits (Theobroma cacao L., var. Trinitario) from the Chontalpa region of the State of Tabasco, Mexico, was kindly supplied by the Local Agricultural Association of Cacao Producers of Huimanguillo. Whey protein hydrolysate (WPH; Hilmar™ 8390, 78% protein on dry basis, 5.5% fat, moisture 3.5%, ash 4.5%, lactose 3.0% and molecular weight distribution of 70.8% < 1000 Da, 12.9% 1000–5000 Da, 6.6% 5000–20,000 Da and 9.5% > 20,000 Da) was supplied by Hilmar Cheese Company (Hilmar, CA, USA). Citric acid, hydrochloric acid (HCl), sodium hydroxide (NaOH), magnesium sulfate heptahydrate (MgSO4·7H2O), sulfuric acid (H2SO4) and ethanol, were analytical grade and purchased from J.T. Baker (Xalostoc, State of Mexico, Mexico). Potassium sulfamate, sodium tetraborate, 3-phenylphenol. Other reagent-grade chemicals were purchased from SigmaAldrich Mexico (Toluca, State of Mexico, Mexico). Deionized water was used in all the experiments. 2.2. Extraction of cacao pod husks pectin (CPHP) Cacao pod was cut lengthwise and seeds were removed manually from the husk. Husks were cut into small pieces, dehydrated in an oven with air circulation (Riossa Digital, HCF-62, Mexico City, Mexico) at 55 °C until achieving constant weight (~ 36 h). Dried pieces were milled (NixtamaticMR, Mexico City, Mexico) using successive sieves of 2 mm and 1 mm. Cacao pod husks ﬂour (CPHF) that passed across the 1 mm sieve was used for the extraction of pectin. CPHP was extracted by acid hydrolysis as proposed by Vriesmann et al. , with slight modiﬁcations. Brieﬂy, 100 g of CPHF were mixed with 2.5 L of citric acid (1:25 w/v) and put in a water bath with constant stirring. Extraction conditions were: pH of 3.0, 85 °C and 90 min extraction time. The resulting extract was cooled to room temperature (23 ± 2 °C) and ﬁltered using a synthetic cloth, then this extract was centrifuged at 8000 × g for 10 min (Centrifuge 5810 R, Eppendorf, AG, Hamburg, Germany) and the precipitate was discarded (impurities). Supernatant was added with 96% ethanol in a 2:1 volume ratio and maintained for 24 h at 4 ± 1 °C, to allow pectin precipitation . Pectin was then separated by ﬁltration through Whatman No. 1 ﬁlter paper and washed twice with 70% ethanol in a 1:1 volume ratio for removal of free sugars, pigments and other impurities. Excess alcohol was removed by centrifugation at 8000 × g for 25 min at 20 °C, and the supernatant was discarded. The pellet was dried at 55 °C in an oven with air circulation until constant weight was achieved. The dried
DM% = V2 (mL)/(V1 (mL) + V2(mL) + V3(mL) − V4(mL)) × 100 (2)
DAmd% = V3 (mL)/(V1 (mL) + V2(mL) + V3(mL) − V4(mL)) × 100 (3)
DAc% = (V4 ×
× 0.05 (mol/L))/((0.500 (g) × 0.821))
× 194.14 (g/mol) × 100
2.3.2. Methoxyl percentage Methoxyl percentage (MeO%) was determined according to Zouambia et al. . MeO is related to DM because the amount of methoxyl groups in 100% of esteriﬁed pectin is 16.32%, the methoxyl percentage was calculated from the following Eq. (5).
MeO% = (16.32/100 ) × DM
2.3.3. Determination of galacturonic acid Galacturonic acid content was estimated by the sulfamate/3-phenylphenol colorimetric assay, reported by Filisetti-Cozzi and Carpita 62
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
. 0.4 mL of CPHP (100 μg mL− 1) were added with 40 μL of 4 M potassium sulfamate solution at pH 1.6, and 2.5 mL of 75 mM sodium tetraborate solution in H2SO4, and the mixture was vortexed for one min and cooled to room temperature in an ice bath. Then the tubes were put into boiling water during 15 min, and the reaction was stopped by cooling in ice-water bath for 1.0–1.5 min. Finally, 80 μL of 0.5% 3-phenylphenol (w/v) in 0.5% NaOH (w/v) was added and the sample was vortexed prior to reading its absorbance at 525 nm in a spectrophotometer (Genesys 10S UV–Vis, Thermo Scientiﬁc, USA). The quantiﬁcation of galacturonic acid was performed, using D-galacturonic acid as standard (Sigma-Aldrich Mexico, Toluca, State of Mexico, Mexico).
2.5. Soluble complexes preparation Aqueous stock solutions (1.0% w/w) of CPHP and WPH were prepared and stored at 4 ± 1 °C during 24 h to ensure their complete hydration. These stock solutions were diluted with deionized water to a desired concentration required for a given experiment. The zeta potential (ζ-potential) of the biopolymers solutions (0.05% w/w) was determined with a Zetasizer Nano ZS90 coupled to the autotitrator MTP-2 (Malvern Instruments Ltd., Malvern, Worcestershire, UK) at pH values ranging between 2.0 and 7.0 at 25 °C. The pH of the solutions was adjusted to the desired value by the addition of either 0.1 N NaOH or 0.1 N HCl. The ζ-potential was determined by measuring the direction and velocity of the dispersion molecules as they moved along the applied electric ﬁeld. The equipment software converted the electrophoretic mobility measurements into ζ-potential values using the Smoluchowski mathematical model. Complexation between oppositely charged biopolymers not only depends on pH, but also on the relative weight ratio between the interacting biopolymers. The pH where the maximum stoichiometric (pHstoich) diﬀerence between the positive ζ-potential of WPH and negative ζ-potential of CPHP occurred was selected as the pH for driving the electrostatic interaction between both biopolymers. In order to determine the weight ratio between WPH and CPHP leading to soluble complexes formation (RWPH-CPHP); CPHP dispersion 10 mL (0.02 mg mL− 1) at pHstoich was transferred to the autotitrator and titrated with WPH dispersion (0.5 mg mL− 1) at pHstoich. Changes in ζpotential and average hydrodynamic diameter (dh) of the WPH-CPHP mixtures were measured as aliquots of ~0.25 mL of WPH were added to the CPHP dispersion. The RWPH-CPHP selected for soluble complex formation was the last point where the hydrodynamic diameter remained practically constant, before commencing to increase sharply.
2.3.4. Determination of protein content Protein content was determined by the assay of Lowry . Initially, 0.5 mL of CPHP (0.01 g/mL) and 0.5 mL of deionized water were put into amber glass tubes. Afterwards 1 mL of solution A (sodium tartrate carbonate, 0.8 N NaOH and 10% sodium dodecyl sulfate) was added and the mixture was vortexed for 1 min and left to stand for 10 min. Subsequently, 0.5 mL of solution B (0.3 N Folin–Ciocalteau reagent) was added to each amber glass tubes, vortexed for 1 min, after which the samples were left to stand for 30 min. Finally, absorbance readings were taken at 750 nm, using bovine serum albumin as standard (Sigma-Aldrich Mexico, Toluca, State of Mexico, Mexico). 2.4. Intrinsic viscosity (η) and estimation of the average viscosimetric molecular weight Intrinsic viscosity [η] determination was realized according to the procedure of Cuevas-Bernardino et al. , with slight modiﬁcations. Stock solution (0.1% w/v) was prepared by dispersing CPHP in deionized water (100 mM NaCl) under magnetic stirring during 30 min at room temperature until full dissolution, and stored at 25 °C for 24 h in order to complete the hydration. This stock solution was diluted in a range of concentration (0.001–0.1 g/100 mL). Diluted samples were vigorously stirred on a vortex mixer and left to equilibrate at least 15 min prior to viscosity measurements. Viscosity was determined with a Physica MCR 301 Dynamic Shear Rheometer (Physica Messtechnik, Stuttgart, Germany) using the DG26.7 concentric cylinders geometry with double gap at a constant speed of 62.1 s− 1 (20 rpm), allowing the sample to stand for 5 min to recover its structure, and for temperature to equilibrate at 25 °C with the help of the Physica TEK 150P Peltier system. Relative (ηrel), speciﬁc (ηsp) and reduced (ηred) viscosities were calculated from the following Eqs. (6)–(8):
ηrel = η1 /η0
ηsp = (η1 /η0 ) − 1
ηred = (η1 /η0 ) − 1 C
2.6. Apparent shear viscosity The apparent shear viscosity of CPHP and SCWPH-CPHP solutions (1.0% w/w) was determined on a rheometer using a concentric cylinder geometry with double-gap and applying a shear rate of 50 s− 1, since it has been reported that this shear rate value is equivalent to that applied in the mouth, and correlates well with the perceived viscosity by consumers . 2.7. Fourier-transform infrared spectroscopy (FT-IR) CPHP, WPH and SCWPH-CPHP were subjected to FT-IR analysis to determine their major functional groups. The FT-IR spectra were obtained using a spectrometer (Frontier FT-IR/FIR, Perkin Elmer, Waltham, MA, USA) equipped with a crystal diamond universal ATR sampling accessory. Approximately 0.2 g of sample were placed on the ATR spectrometer attachment and pressed with the ATR head. Measurements were obtained over the range of 4000 to 400 cm− 1 at a resolution of 4 cm− 1. There were 40 scans per sample which were integrated to obtain mean values of the spectrum. Fourier self-deconvolution and second derivative resolution enhancement were applied to increase the spectral resolution with the equipment software.
where η1 is the viscosity of the pectin solution, η0 is the viscosity of the solvent (100 mM NaCl solution) and C is the pectin concentration. Intrinsic viscosity [η] was calculated by linearly extrapolating the reduced viscosity to zero concentration. Intrinsic viscosity is related to the molecular weight [Mw] through the Mark-Houwink-Sakurada Eq. (9):
[η] = k′[Mw]α
2.8. Dynamic interfacial tension Dynamic of interfacial adsorption of CPHP (1.0% w/w) and SCWPH(1.0% w/w) at the canola oil-water interface was determined by monitoring the evolution of interfacial tension (γ) with time (θ). The method used was that described by Tang and Shen , with slight modiﬁcations. An optical contact angle meter, OCA-20, equipped with oscillating drop accessory ODG-20 (Dataphysics Instruments GmbH, Filderstadt, Germany) was used. One drop of approximately 40 μL of CPHP and SCWPH-CPHP were automatically formed with the aid of a syringe into a glass cuvette containing the puriﬁed canola oil phase. The
where k' and α are empirical constants, which depend on temperature, as well as the polymer-solvent system and correspond to values of 5.08 × 10− 3 ± 2 × 10− 4 and 0.71 ± 0.02 dL/g, respectively . It should be noted that these constants can be used to determine the average viscosimetric molecular weight of pectin if the system conditions are maintained (25 °C and a solution of 100 mM NaCl as solvent). 63
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
shape of the drop was analyzed to record changes in interfacial tension over a period of 10,800 s (3.0 h) with a CCD camera. Experiments were carried out at 25 °C.
Table 1 Physicochemical characteristics of pectin extracted from the cacao pod husks (CPHP). CPHP
2.9. Preparation and characterization of emulsions
DM (%) DAmd (%) DAc (%) MeO (%) Galacturonic acid (%) Protein (%) Moisture (%) Yield (g/100 g) Apparent viscosity (Pa·s)a Intrinsic viscosity (dL/g) Molecular weight (viscosimetric) (kDa)
2.9.1. Preparation Oil-in-water emulsions were prepared using CPHP and SCWPH-CPHP (1.0% w/w) at pH 3.25 as the continuous phase (w) and canola oil as oily phase (o). The o/w emulsions had a dispersed phase mass fraction of 0.1. The o/w emulsions were coded as Ex, where x stands for the emulsifying agent used. Emulsions were prepared by incorporating the dispersed phase drop-wise with continuous agitation into the continuous phase with the help of a high shear homogenizer (Ultra-Turrax® T50 basic IKA Works, Inc., Wilminton, USA), operated at 8000 rpm for 3 min to form coarse emulsion. Finally, the coarse emulsions were passed through a highpressure homogenizer (Microﬂuidics® M-110P, Newton Massachusetts, USA) operated at 100 MPa for three cycles. An ice bath was used for avoiding temperature increase during emulsion formation. The emulsions were stored at 4 ± 1 °C prior to further analysis.
83.22 ± 0.96 0.62 ± 0.09 10.20 ± 0.33 13.58 ± 0.16 72.01 ± 0.20 3.68 ± 0.22 4.94 ± 0.30 6.18 ± 0.31 0.026 ± 7.27 × 10− 5 8.82 255.85
The percentages are on dry basis. a Determined at a shear rate of 50 s− 1 and at a concentration of 1.0% w/w.
DM value was 83.22%, so CPHP can be classiﬁed as a high methoxyl pectin (DM > 50%) [1,3,39]. Fig. 1 shows the schematic representation of CPHP. It has been reported that methoxyl groups on pectin backbone can act as a driving force for the molecular diﬀusion mechanism to oil-in-water interface during emulsions formation, due to its hydrophobic nature [8,40]. DAmd (0.62%) of CPHP is too low for achieving an eﬃcient release of aromatic compounds (alcohols, ketones, aldehydes, and esters), as Kim et al.  reported that an amidation degree of 14% or more was required for achieving this purpose. DAc of CPHP was 10.20%, and according to Alba and Kontogiorgos , pectins with a DAc of at least 10%, may show good emulsifying and interfacial activities, such as in the case of sugar beet pectins [10,42,43]. Vriesmann and Petkowicz  reported that CPHP with 17% DAc possessed good gelling properties. Protein content (3.68%) of CPHP was lower than 8.6% reported by Vriesmann et al. .
2.9.2. Characterization of emulsions The area-volume mean diameter (d3.2) of the freshly prepared emulsions was veriﬁed using a static laser diﬀraction particle size analyzer (Malvern Mastersizer 3000, Malvern Instruments, Ltd., Worcestershire, UK). Refractive indexes of the dispersed and continuous phases used in the calculations were 1.466 and 1.330, respectively, determined with a refractometer (ABBE 5 refractometer, Model 44-501; American Optical Co., USA). The change in d3.2 of Ex was monitored at 0, 1, 7, 14, 21 and 28 days. Creaming rate of the emulsions was evaluated in a LUMiSizer centrifuge (LUM GmbH, Berlin, Germany), an instrument that uses centripetal force to accelerate the instability of emulsions due to aggregation phenomena . Instrumental parameters used for the measurements were as follows: volume, 0.4 mL of emulsion in the cell; rotation speed of 3000 rpm; 255 measurements determined at time intervals of 30 s and temperature of 25 °C . Creaming rate was provided by the equipment software, and provides a measure of the stability of the emulsion: the higher the rate of creaming, the lower the emulsion stability . ζ-Potential of the freshly prepared emulsions was determined with a Zetasizer Nano ZS90 equipment. Samples of Ex, were diluted in deionized water (ratio of 1:100 v/v) and then ﬁlled into the test cell and placed on the measuring equipment.
3.2. Intrinsic viscosity and viscosimetric molecular weight estimation Behavior of the reduced viscosity vs concentration of dilute CPHP solutions was studied in order to obtain the intrinsic viscosity [η] (Fig. 2). Upon dilution in pure water, polyelectrolytes such as gum Arabic and pectin initially exhibit a decrease in reduced viscosity (ηred) followed by an increase, due to a coil expansion by the mutual repulsion between like charges attached to the coil . Addition of sodium chloride is commonly used to reduce or eliminate conformational changes with concentration of polyelectrolytes, and a linear dependence of the reduced viscosity over polyelectrolyte concentration occurs . This is because Na+ counterions screen the ionic interactions and molecules adopt a more compact conformation in solution and thus, intrinsic viscosity [η] value decreases . [η] measures the hydrodynamic volume per gram of macromolecular substance at inﬁnite dilution, and is obtained when the ηred data is extrapolated to “zero” concentration, where theoretically the molecular interactions of the polymers are suppressed. [η] is a characteristic related to the molecular weight and the conformation of polymers . Conformations of pectin include random coils, spheres, rigid rod-like, and may aﬀect the adsorption mechanism at the oil-water interface [20,49]. [η] and viscosimetric molecular weight (Mw) of CPHP were 8.82 dL/g and 255.85 kDa, respectively. These values are higher than those reported by Yapo and Koﬃ  for cacao pod husks pectin which were of 1.62–3.04 dL/g for [η] and of 43–82 kDa for Mw. The diﬀerences can be attributed to extraction method, origin, variety, and edafoclimatic conditions.
2.10. Statistical analysis All experiments were done in triplicate from 3 independent experiments using a randomized experimental design and values were expressed as mean values ± SD. Data were subjected to simple classiﬁcation analysis of variance and in pertinent cases to Tukey's mean comparison analysis. Signiﬁcance was established at p ≤ 0.05. Data analysis was performed with the Statgraphics Plus software (Statistical Graphics Centurion XVI (StatPoint Technologies, Inc., Warrenton, Virginia, USA). 3. Results and discussion 3.1. Physicochemical characteristics of cacao pod husks pectin
3.3. ζ-Potential of stock dispersions and formation of SCWPH-CPHP
CPHP yield was of 6.18 g/100 g in dry basis (d.b.), which was within the range of 2.64 to 10.6 g/100 g reported by several authors [17,18,20]. The physicochemical characteristics of CPHP are presented in Table 1. CPHP had a galacturonic acid content higher than 65%, which is the minimum requirement for commercial applications .
ζ-Potential variation with pH for CPHP and WPH dispersions is shown in Fig. 3. ζ-Potential values for CPHP dispersions were negative throughout the pH range studied, due to the low pKa values of their 64
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
Reduced Viscosity (dL/g)
Fig. 1. Schematic representation of the structure of the cacao pods husk pectin (CPHP).
carboxyl groups. ζ-potential values presented by CPHP were in accordance with those reported by Jones et al.  for high methoxyl pectins. The carboxylic groups (eCOOH) present at low pH were converted to carboxylate groups (eCOO−) as pH increased, and the magnitude of negative ζ-potential value increased. The maximum slope of the ζ-potential curve of the CPHP occurred in a pH range of 3.0 to 4.0, and can be related to the pKa of CPHP solutions . For WPH, ζ-potential values varied between 30.0 ± 0.75 mV at pH 2.0 to − 30.7 ± 1.2 mV at pH 7.0. A zero ζ-potential value occurred at the isoelectric point (pI; pH of 4.27). The negative ζ-potential values that occurred at pH values > pI can be attributed to the ionization of the carboxylic groups (eCOOH) into carboxylate groups (eCOO−), while the positive ζ-potential values at pH < pI are due to the protonation of the amino moieties (eNH2) giving rise to ammonium groups (eNH4+). pH of the medium strongly aﬀected the charge density of the studied biopolymers, which in turn aﬀect the strength of complexation or interaction between them. According to the interaction window between positively charged WPH and negatively charged CPHP, the pH where the maximum stoichiometric diﬀerence occurred was 3.25, therefore this value was used as pHstoich. ζ-Potential and hydrodynamic diameter (dh) measurements were used to provide information about the inﬂuence of the weight ratio between WPH and CPHP (RWPH-CPHP) on the formation of soluble complexes. These parameters were measured as a CPHP dispersion (0.02 mg mL− 1) was titrated with a WPH dispersion (0.5 mg mL− 1) at pH 3.25. Initially the CPHP dispersion was completely transparent and the pectin molecules exhibited a dh of 2173 nm and a ζ-potential of − 20.83 mV (Fig. 4). By adding WPH dispersion to CPHP dispersion the progressive appearance of two complexation main phases was revealed: (1) the ﬁrst phase (called region A) comprised between R0.24:1 to R5:1 where the dh of the WPH-CPHP system decreased slightly, after which it reached a plateau with values around of 821 nm, while the ζ-potential values varied from − 19.96 mV to − 10.38 mV, indicating that the negative charge of the system decreased. In this region the appearance of the WPH-CPHP system was of a uniformly turbid dispersion. The decrease of the CPHP hydrodynamic diameter could be due to the contraction of the pectin molecule, which becomes less expanded as WPH interacts with the carboxylic groups of the polysaccharide . Not all of the negatively charged CPHP moieties are neutralized by the positively charged WPH moieties, so that the complexes formed possess a net negative charge and thus remain soluble in the bulk of the
12 y= 8.823 + 44.350x 2 R = 0.962 [η]= 8.823 dL/g
9 6 3 0 0.00
100 mM NaCl Linear Fit of 100 mM NaCl
Concentration (g/dL) Fig. 2. Reduced viscosity vs concentration of cacao pods husk pectin (CPHP) dispersed in 100 mM NaCl aqueous solution. The solid line shows a linear relationship between reduced viscosity and pectin concentration.
Fig. 3. ζ-Potential versus pH proﬁles of WPH (▲) and CPHP (■) at 0.05% w/w.
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
SCWPH-CPHP spectrum showed displaced peaks with diﬀerent intensities and in some cases the appearance and/or overlap of new absorption signals, presented wave vibrations belonging to the spectral regions of CPHP at 2915, 1734 and 1250 cm− 1, and of WPH at 1630, 1535 and 1240 cm− 1. The absorption in amide I region is considered the most useful for FT-IR analysis of the secondary structure of proteins, and its location depends on the conformation of the protein structure, same that determines its chemical reactivity, intermolecular interactions, and functional properties such as solubility, water holding capacity, gelation, foaming, and emulsiﬁcation . In this case, the amide I peak for WPH was observed at 1630 cm− 1, which has been related to random coil type structures with more entropically favorable conformations, which facilitates the complexation process between the biopolymers . As a result of the biopolymer interaction, FT-IR of SCWPH-CPHP changed signiﬁcantly in the carbonyl-amide region. The eNH3+ groups (Amide B) for WPH and asymmetric and symmetric eCOO– stretching vibration at 1607 cm− 1 and 1423 cm− 1 for CPHP disappeared, respectively, indicating the electrostatic interaction between the amine groups of WPH (NH3+) and carboxyl groups of CPHP (eCOO−) . At the same time, the soluble complex showed an amide A peak at a lower wavenumber (3270 cm− 1) than WPH, indicating some hydrogen bindings between amino or eOH of WPH and eOH of CPHP took place . Therefore, the manifestations of this type of vibrations in the wavenumbers mentioned permitted to establish changes in the original conformation of the biopolymers, suggesting that the complexing between WPH and CPHP was successful. A schematic representation of SCWPH-CPHP derived from the above observations is given in Fig. 6.
Fig. 4. Evolution of the ζ-potential and hydrodynamic diameter as function of the weight ratio (RWPH-CPHP) between WPH and CPHP at pH 3.25.
aqueous phase ; and (2) the second phase (called region B) comprised between R5.5:1 to R8.24:1 was characterized by a drift in the ζpotential values towards zero and by a sharp upward increase in dh reaching values of up to 14,747 nm. These results are indicative of the progressive neutralization of the negative charges of the CPHP by increased added amounts of WPH, which resulted in association of the soluble complexes in larger and insoluble complexes (complex coacervates) as was evidenced by the macroscopic phase separation . Thus, from these results a R5:1 was chosen for obtaining the SC. 3.4. Fourier transform infrared spectroscopy (FT-IR) FT-IR spectra of CPHP, WPH and SCWPH-CPHP are shown in Fig. 5. The two principal absorbance peaks that dictate the major functional properties of CPHP occur approximately at 1725 and 1607 cm− 1, which are attributed to the esteriﬁed carboxyl groups and to the ionic carboxyl groups (eCOO−), respectively [53–55]. The acetyl group has multiple wavenumbers, the most important being C]O stretching peaks, around 1720 cm− 1, the CeH stretching vibration of the CH3 group between 2960 and 2870 cm− 1 and the CeO stretching vibration around 1250 cm− 1 and 1255 cm− 1 [56,57]. The above mentioned absorption bands are characteristic of chemically modiﬁed polysaccharides by acetylation [58,59] and they are present in the CPHP spectrum, indicating that this molecule has this functional group which is consistent with the data reported in Table 1. WPH spectrum, showed absorbance peaks around 1630 cm− 1 corresponding to C]O stretching of amide I, around 1535 cm− 1 corresponding to NeH bend of the amide II and ﬁnally around 1240 cm− 1 corresponding to CeN stretching and NeH bend of the amide III [60–63].
3.5. Dynamic interfacial tension The adsorption of molecules with surface-active capacity at the oilwater interface is the most important step in the formation of emulsions . During the adsorption process, these molecules undergo conformational changes as they interact with the interface . The dependence of the interfacial tension (γ) as a function of time of CPHP (1.0% w/w) and SCWPH-CPHP (1.0% w/w) at the canola oil-water interface is shown in Fig. 7. The interfacial tension of the deionized water was 29.5 ± 0.50 mN/m, whereas that of CPHP was 25.20 ± 0.43 mN/m after 10 s. This decrease may be related to structural components of CPHP as: i) hydrophobic groups (methyl ester and acetyl), ii) molecular conformation and iii) the presence of protein residues. These
Fig. 5. FT-IR spectra of CPHP, WPH and SCWPH-CPHP.
Fig. 6. Schematic representation of the structure of SCWPH-CPHP.
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
22 20 18 16 14 12 0
Time (s) Fig. 7. Interfacial tension adsorption dynamics at the oil-water interface of CPHP (■) and SCWPH-CPHP (○) at 1.0% w/w.
components acted as hydrophobic anchors and facilitated the adsorption of CPHP at the interface, resulting in the reduction of interfacial tension [12,39,40,42]. The initial interfacial tension (10 s) of SCWPH-CPHP was 22.85 ± 0.30 mN/m and was lower than that of CPHP after 10 s. The increase in the amino groups acted as a driving force for diﬀusion to the interface, indicating that the SCWPH-CPHP molecules diﬀused to and anchored at the interface at a faster rate than those of CPHP, saturating faster the interfacial monolayer. The subsequent relative slow drop in the interfacial tension at longer times of CPHP and SCWPH-CPHP can be caused by the reconformation of the adsorbed molecules in the interface . The adsorption kinetics of the biopolymers were determined from surface pressure changes (π) over time, which was derived from the data of Fig. 7. The main stages of adsorption kinetics that can be deﬁned based on the surface pressure-time curves proﬁles are as follows: (i) diﬀusion, (ii) penetration and (iii) rearrangement of molecules at the oil-water interface, multilayer formation and possibly interfacial gelling, which give rise to diﬀusion (kdiﬀ), penetration (kpen) and molecular rearrangement (krea) rate constants, respectively . During the ﬁrst stage, at relatively low surface pressures a modiﬁed form of the Ward and Tordai  equation can be used to correlate the change in surface pressure with time (Eq. 10): 1
π = 2C0 KT(D θ/3.14)
Fig. 8. a) Dependence of surface pressure (π) as a function of the square root of time (s0.5). The solid-solid line depicts the linear slope of the curves where the adsorption is diﬀusion-controlled (kdiﬀ). b) Plot of ln (π10800 − πθ)/(π10800 − π0) versus θ. The continuous solid line depicts the ﬁrst slope corresponding to the ﬁrst-order rate constants of adsorption/penetration (kpen), while the second slope corresponds to the ﬁrst-order rate constants of structural rearrangement (krea). For CPHP (□) and SCWPH-CPHP (○) at the oilwater interface at 1.0% w/w concentration.
Table 2 Parameters of the adsorption dynamics of the biopolymers under study at the oil-water interface.
where C0 is the initial biopolymer concentration in the aqueous phase, K is the Boltzmann constant, T is the absolute temperature, D is the diﬀusion coeﬃcient and θ is the adsorption time. If diﬀusion at the interface controls the adsorption process, a plot of π against θ½ will be linear and the slope of this plot will be kdiﬀ, . From Fig. 8a it can be seen that for both CPHP and SCWPH-CPHP the diﬀusion controlled adsorption occurred within 90 s. kdiﬀ values for CPHP and SCWPH-CPHP are given in Table 2. SCWPH-CPHP exhibited a steeper slope than CPHP. This behavior may be related to the amino group's content of SCWPH-CPHP (protein content of 54.39 ± 1.47%) which was 14.7 times greater than that of CPHP. Additionally, the apparent viscosity at 50 s− 1 of SCWPH−5 Pa·s) was 3.5 times lower than that of CPHP (0.0074 ± 3.10 × 10 CPHP, so that the molecules of the former encountered a lower resistance to their mobility, and were capable of migrating faster to the oil-water interface. After the sharp initial adsorption period (≤ 90 s), the rate of adsorption of CPHP and SCWPH-CPHP slowed down up to 10,800 s, and the π − θ data within this time interval can be analyzed with the following ﬁrst-order phenomenological Eq. (11) , in order to obtain kpen and krea constants:
Type of biopolymer
kdiﬀ (mN/m− 1 s0.5)
kpen × 104 (s− 1)
krea × 104 (s− 1)
0.41 ± 0.09 0.81 ± 0.14
3.45 ± 0.02 4.99 ± 0.02
15.90 ± 1.03 13.40 ± 0.22
CPHP: cacao pod husks pectin; SCWPH-CPHP: soluble complex between CPHP and whey protein hydrolysate (WPH); diﬀusion (kdiﬀ), penetration (kpen) and rearrangement (krea) constants.
ln(π10800 − πθ/ π10800 − π0 ) = −ki θ
where π10800, πθ, π0, are the surface pressure values at the experimental ﬁnal adsorption time (10,800 s), of each step (θ) and at the initial time (90 s), respectively, and ki is the ﬁrst-order rate constant. These plots usually yield two linear slopes, where the ﬁrst slope refers to kpen, and the second slope krea. The plot of ln [(π10800 − πθ) / (π10800 − π0)] against the time for SCWPH-CPHP and CPHP showed similar proﬁles (Fig. 8b). SCWPH-CPHP exhibited a higher value of kpen (Table 2) indicative that the complex molecules could penetrate the monolayer at the interface more easily than those of CPHP, probably because of the higher aﬃnity (higher hydrophobicity) of its molecular segments to the oil phase. On the other hand, CPHP displayed a higher value for krea 67
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
droplets than around ECPHP droplets. Finally, ECPHP showed a signiﬁcantly higher creaming index (9.72 ± 0.33%) than EWPH-CPHP (3.53 ± 0.55%), despite that EWPHCPHP displayed lower apparent viscosity (0.143 ± 0.008 Pa·s) and lower ζ-potential (− 25.36 ± 0.42 mV) than ECPHP (0.250 ± 0.001 Pa·s and −37.32 ± 0.28 mV, respectively). These results seem to pinpoint that the higher concentration of smaller sized droplets in EWPH-CPHP enhanced the formation of 3-D network, where the steric stabilization term was the dominant stabilizing mechanism , and where ζ-potential of the droplet and the apparent viscosity of the emulsion had little bearing on emulsion stability. 4. Conclusions Cacao pod husks agroindustrial wastes can be used for obtaining pectin by using a simple environmental friendly extraction process. The cacao pod husks pectin (CPHP) showed both surface active and emulsifying activities. Modiﬁcation of CPHP by its complexing with whey protein hydrolysate (WPH) improved signiﬁcantly the surface active and emulsifying activities. Oil-in-water emulsion utilizing WPH-CPHP soluble complex (SCWPH-CPHP) as emulsiﬁer/stabilizer producing nanometric droplet sizes, which did not show signiﬁcant changes during 28 days of storage, and displayed a low creaming index under accelerated centrifugation testing. Thus, an important contribution of this work was to provide a simple and eﬃcient methodology for imparting superior surface active and emulsifying activities to CPHP, and the knowledge derived from this study could broaden CPHP application in the food industry, and contribute to reduce contamination problems associated with cacao processing byproducts.
Fig. 9. Variation of the area-volume mean diameter (d3,2) of the oil droplets during 28 days of storage at 4 ± 1 °C. ECPHP (■) and EWPH-CPHP (■) at 1% w/w. Diﬀerent lowercase and uppercase letters indicate signiﬁcant diﬀerences between means (p ≤ 0.05).
than SCWPH-CPHP, indicative that the latter molecules packing at the interface was higher than that of the former molecules, which restricted their freedom for rearrangement .
3.6. Formation and stabilization of oil-water emulsions The size of O/W emulsion droplets is determined by the two fundamental processes that occur during its preparation: the fragmentation of the dispersed phase into small droplets and the coalescence of the recently formed droplets. The emulsifying/stabilizing agents have effects on both processes, by: a) the reduction of the interfacial tension, which promotes the rupture of the dispersed phase into small droplets and b) the formation of an interfacial biopolymer ﬁlm, which prevents the phenomenon of coalescence . Fig. 9 shows the d3,2 evolution of the O/W emulsions prepared with CPHP (1% w/w) and SCWPH-CPHP (1% w/w), stored at 4 ± 1 °C for 28 days. EWPH-CPHP displayed oil droplets with signiﬁcantly lower initial d3,2 (86.98 ± 4.0 nm) than ECPHP (113.2 ± 0.5 nm). EWPH-CPHP did not show a signiﬁcant change in droplet size (90.36 ± 01.3 nm), while ECPHP suﬀered a signiﬁcant increase (162.0 ± 3.61 nm) during the 28 days of storage time. Several authors have reported the formation of O/W emulsions stabilized with pectin from various botanical sources, such as apple, citrus, sugar beet and hawthorn (conc. 0.5–1.5%) and droplet sizes in the range of 0.4–20 μm [11,16,55,71,72]. Notice that the mean droplet sizes obtained in this work were in the nanometric scale while those reported in the works cited above fell basically within the micrometric scale. Yapo and Koﬃ  reported that pectin from cacao pod husks exhibited good emulsifying and emulsion-stabilizing activities, but did not provide details of the droplet size of the emulsions. The possible explanations involved for the better emulsifying and stabilizing performance of SCWPH-CPHP in comparison to CPHP are the following: (a) SCWPH-CPHP displayed a higher kdiﬀ due to its higher hydrophobic character than CPHP, so that the molecules diﬀused and anchored more rapidly at the interface, forming initial smaller droplet sizes; and (b) Once small droplets have been formed, the key factor aﬀecting emulsion long-term stability is how the adsorbed molecules conform at the interface, and if they are able of forming thick steric stabilizing layers. The higher kpen and lower krea displayed by SCWPHCPHP in comparison to CPHP, indicated than the improved penetration and packing occurred as a result of the smaller hydrodynamic diameter and lower negative surface charges showed by the complex. The overall eﬀect was the formation of a bulkier interfacial layer around EWPH-CPHP
Acknowledgements This research was partially supported by the Consejo Nacional de Ciencia y Tecnología (CONACyT) of Mexico, through projects 236500 and 410175. References  F. Munarin, M.C. Tanzi, P. Petrini, Review: advances in biomedical applications of pectin gels, Int. J. Biol. Macromol. 51 (2012) 681–689.  L. Zhang, Z. Shi, W. Shangguan, Y. Fang, K. Nishinari, G.O. Phillips, F. Jiang, Emulsiﬁcation properties of sugar beet pectin after modiﬁcation with horseradish peroxidase, Food Hydrocoll. 43 (2014) 107–113.  X. Hua, K. Wang, R. Yang, J. Kang, J. Zhang, Rheological properties of natural lowmethoxyl pectin extracted from sunﬂower head, Food Hydrocoll. 44 (2015) 122–128.  R. Lutz, A. Aserin, L. Wicker, N. Garti, Structure and physical properties of pectins with block-wise distribution of carboxylic acid groups, Food Hydrocoll. 23 (2009) 786–794.  C. Kyomugasho, S. Christiaens, A. Shpigelman, A.M. Van Loey, M.E. Hendrickx, FTIR spectroscopy, a reliable method for routine analysis of the degree of methylesteriﬁcation of pectin in diﬀerent fruit- and vegetable-based matrices, Food Chem. 176 (2015) 82–90.  C.D. May, Industrial pectins: sources, production and applications, Carbohydr. Polym. 12 (1990) 79–99.  B.R. Thakur, R.K. Singh, A.K. Handa, M.A. Rao, Chemistry and uses of pectin–a review, Crit. Rev. Food Sci. Nutr. 37 (1997) 47–73.  K. Burapapadh, H. Takeuchi, P. Sriamornsak, Novel pectin-based nanoparticles prepared from nanoemulsion templates for improving in vitro dissolution and in vivo absorption of poorly water-soluble drug, Eur. J. Pharm. Biopharm. 82 (2012) 250–261.  E.D. Ngouémazong, S. Christiaens, A. Shpigelman, A. Van Loey, M. Hendrickx, The emulsifying and emulsion-stabilizing properties of pectin: a review, Compr. Rev. Food Sci. Food Saf. 14 (2015) 705–718.  J. Leroux, V. Langendorﬀ, G. Schick, V. Vaishnav, J. Mazoyer, Emulsion stabilizing properties of pectin, Food Hydrocoll. 17 (2003) 455–462.  M.I. Guerra-Rosas, J. Morales-Castro, L.A. Ochoa-Martínez, L. Salvia-Trujillo, O. Martín-Belloso, Long-term stability of food-grade nanoemulsions from high methoxyl pectin containing essential oils, Food Hydrocoll. 52 (2016) 438–446.  U.S. Schmidt, L. Schütz, H.P. Schuchmann, Interfacial and emulsifying properties of citrus pectin: interaction of pH, ionic strength and degree of esteriﬁcation, Food Hydrocoll. 62 (2017) 288–298.  P.A. Williams, C. Sayers, C. Viebke, C. Senan, Elucidation of the emulsiﬁcation properties of sugar beet pectin, J. Agric. Food Chem. 53 (2005) 3592–3597.
Reactive and Functional Polymers 123 (2018) 61–69
D. Trujillo-Ramírez et al.
(Theobroma cacao L.) forms gel, Food Hydrocoll. 33 (2013) 58–65.  L.C. Vriesmann, R.D.M.C. Amboni, C.L.O. Petkowicz, Cacao pod husks (Theobroma cacao L.) composition and hot-water-soluble pectins, Ind. Crop. Prod. 34 (2011) 1173–1181.  W.M. Pasika, Polysaccharide polyelectrolytes, in: P.A. Sanford, A. Laskin (Eds.), Extracellular Microbial Polysaccharides, American Chemical Society, Washington, D.C., 1977, pp. 128–143.  C.E. Brunchi, S. Morariu, M. Bercea, Intrinsic viscosity and conformational parameters of xanthan in aqueous solutions: salt addition eﬀect, Colloids Surf. B: Biointerfaces 122 (2014) 512–519.  L. Yang, L.-M. Zhang, Chemical structural and chain conformational characterization of some bioactive polysaccharides isolated from natural sources, Carbohydr. Polym. 76 (2009) 349–361.  C.M. Liu, X.J. Guo, R.H. Liang, W. Liu, J. Chen, Alkylated pectin: Molecular characterization, conformational change and gel property, Food Hydrocoll. 69 (2017) 341–349.  O.G. Jones, U. Lesmes, P. Dubin, D.J. McClements, Eﬀect of polysaccharide charge on formation and properties of biopolymer nanoparticles created by heat treatment of β-lactoglobulin–pectin complexes, Food Hydrocoll. 24 (2010) 374–383.  F. Weinbreck, R. de Vries, P. Schrooyen, C.G. de Kruif, Complex coacervation of whey proteins and gum arabic, Biomacromolecules 4 (2) (2003) 293–303.  H. Espinosa-Andrews, K.E. Enríquez-Ramírez, E. García-Márquez, C. RamírezSantiago, C. Lobato-Calleros, E.J. Vernon-Carter, Interrelationship between the zeta potential and viscoelastic properties in coacervates complexes, Carbohydr. Polym. 95 (2013) 161–166.  A. Fellah, P. Anjukandi, M.R. Waterland, M.A.K. Williams, Determining the degree of methylesteriﬁcation of pectin by ATR/FT-IR: methodology optimisation and comparison with theoretical calculations, Carbohydr. Polym. 78 (2009) 847–853.  E. Pretsch, P. Bühlmann, M. Badertscher, Structure Determination of Organic Compounds. Tables of Spectral Data, fourth ed., Springer, Berlin, 2009.  H. Chen, S. Qiu, J. Gan, Y. Liu, Q. Zhu, L. Yin, New insights into the functionality of protein to the emulsifying properties of sugar beet pectin, Food Hydrocoll. 57 (2016) 262–270.  J.F. Mano, D. Koniarova, R.L. Reis, Thermal properties of thermoplastic starch/ synthetic polymer blends with potential biomedical applicability, J. Mater. Sci. Mater. Med. 14 (2003) 127–135.  D. Karnik, J. Jung, S. Hawking, L. Wicker, Sugar beet pectin fractionated using isopropanol diﬀers in galacturonic acid, protein, ferulic acid and surface hydrophobicity, Food Hydrocoll. 60 (2016) 179–185.  J.G. Salcedo-Mendoza, M.C. Rodríguez-Lora, J.A. Figueroa-Flórez, Eﬀect of acetylation on structural and functional properties of starches from cassava (Manihot esculenta Crantz) and yam (Dioscorea alata cv. Diamante 22), Rev. Mex. Ing. Quim. 15 (3) (2016) 787–796.  J. Li, X. Hu, X. Li, Z. Ma, Eﬀects of acetylation on the emulsifying properties of Artemisia sphaerocephala Krasch. polysaccharide, Carbohydr. Polym. 144 (2016) 531–540.  M. Carbonaro, A. Nucara, Secondary structure of food proteins by Fourier transform spectroscopy in the mid-infrared region, Amino Acids 38 (2010) 679–690.  L.G. Gómez-Mascaraque, B. Miralles, I. Recio, A. López-Rubio, Microencapsulation of a whey protein hydrolysate within micro-hydrogels: impact on gastrointestinal stability and potential for functional yoghurt development, J. Funct. Foods 26 (2016) 290–300.  J. Zhu, X. Sun, S. Wang, Y. Xu, D. Wang, Formation of nanocomplexes comprising whey proteins and fucoxanthin: characterization, spectroscopic analysis, and molecular docking, Food Hydrocoll. 63 (2017) 391–403.  F. López-García, C. Jiménez-Martínez, D. Guzmán-Lucero, A. Maciel-Cerda, R. Delgado-Macuil, D. Cabrero-Palomino, E. Terrés-Rojas, I. Arzate-Vázquez, Physical and chemical characterization of a biopolymer ﬁlm made with corn starch and nopal xoconostle (Opuntia joconsotle) mucilage, Rev. Mex. Ing. Quim. 16 (1) (2017) 147–158.  D.J. McClements, Food Emulsions – Principles, Practices, and Techniques, second ed., (2004) (New York).  S.L. Turgeon, S.I. Laneuville, Protein plus polysaccharide coacervates and complexes: from scientiﬁc background to their application as functional ingredients in food products, in: S. Kasapis, I.T. Norton, J.B. Ubbink (Eds.), Modern Biopolymer Science: Bridging the Divide between Fundamental Treatise and Industrial Application, Academic Press, San Diego, 2009, pp. 327–363.  M. Anvari, D. Chung, Dynamic rheological and structural characterization of ﬁsh gelatin – gum arabic coacervate gels cross-linked by tannic acid, Food Hydrocoll. 60 (2016) 516–524.  J.M. Rodríguez-Patino, A.M.R. Pilosof, Protein-polysaccharide interactions at ﬂuid interfaces, Food Hydrocoll. 25 (2011) 1925–1937.  A.F.H. Ward, L. Tordai, Time dependence of boundary tensions of solutions, J. Chem. Phys. 14 (1946) 353–361.  D.E. Graham, M.C. Philips, Proteins at liquid interfaces: I. Kinetics of adsorption and surface denaturation, J. Colloid Interface Sci. 70 (1979) 403–414.  L.L. Lobo, A. Svereika, Coalescence during emulsiﬁcation. 2. Role of small molecule surfactants, J. Colloid Interface Sci. 261 (2003) 498–507.  K. Burapapadh, M. Kumpugdee-Vollrath, D. Chantasart, P. Sriamornsak, Fabrication of pectin-based nanoemulsions loaded with itraconazole for pharmaceutical application, Carbohydr. Polym. 82 (2010) 384–393.  H.M. Chen, X. Fu, Z.G. Luo, Esteriﬁcation of sugar beet pectin using octenyl succinic anhydride and its eﬀect as an emulsion stabilizer, Food Hydrocoll. 49 (2015) 53–60.
 T. Funami, G. Zhang, M. Hiroe, S. Noda, M. Nakauma, I. Asai, M.K. Cowman, S. AlAssaf, G.O. Phillips, Eﬀects of the proteinaceous moiety on the emulsifying properties of sugar beet pectin, Food Hydrocoll. 21 (2007) 1319–1329.  B.M. Yapo, C. Robert, I. Etienne, B. Wathelet, M. Paquot, Eﬀect of extraction conditions on the yield, purity and surface properties of sugar beet pulp pectin extracts, Food Chem. 100 (2007) 1356–1364.  J.C. Cuevas-Bernardino, C. Lobato-Calleros, A. Román-Guerrero, J. AlvarezRamirez, E.J. Vernon-Carter, Physicochemical characterisation of hawthorn pectins and their performing in stabilising oil-in-water emulsions, React. Funct. Polym. 103 (2016) 63–71.  L.C. Vriesmann, R.F. Teóﬁlo, C.L.O. Petkowicz, Extraction and characterization of pectin from cacao pod husks (Theobroma cacao L.) with citric acid, LWT-Food Sci. Technol. 49 (1) (2012) 108–116.  H. Bazarte, E. Sangronis, E. Unai, La cáscara de cacao (Theobroma cacao L.): Una posible fuente comercial de pectinas, Arch. Latinoam. Nutr. 58 (2008) 64–70.  International Cocoa Organization (ICCO), Assessment of world cocoa bean stocks for 2014–15, https://www.icco.org/home/latest-news.html, (2016) , Accessed date: 1 September 2017.  B.M. Yapo, K.L. Koﬃ, Extraction and characterization of gelling and emulsifying pectin fractions from cacao pod husk, J. Food Nutr. Res. 1 (4) (2013) 46–51.  C. Schmitt, S.L. Turgeon, Protein/polysaccharide complexes and coacervates in food systems, Adv. Colloid Interf. Sci. 167 (2011) 63–70.  N.Y. Hernández-Marín, C. Lobato-Calleros, E.J. Vernon-Carter, Stability and rheology of water-in-oil-in-water multiple emulsions made with protein-polysaccharide soluble complexes, J. Food Eng. 119 (2013) 181–187.  H. Salminen, J. Weiss, Electrostatic adsorption and stability of whey protein-pectin complexes on emulsion interfaces, Food Hydrocoll. 35 (2014) 410–419.  J.P. Pérez-Orozco, E. Barrios-Salgado, A. Román-Guerrero, R. Pedroza-Islas, Interaction of mesquite gum-chitosan at the interface and its inﬂuences on the stability of multiple emulsions W1/O/W2, Rev. Mex. Ing. Quim. 10 (3) (2011) 487–499.  D.J. McClements, J. Rao, Food-grade nanoemulsions: formulation, fabrication, properties, performance, biological fate, and potential toxicity, Crit. Rev. Food Sci. Nutr. 51 (4) (2011) 285–330.  I. Gülseren, M. Corredig, Interactions at the interface between hydrophobic and hydrophilic emulsiﬁers: polyglycerol polyricinoleate (PGPR) and milk proteins, studied by drop shape tensiometry, Food Hydrocoll. 29 (2012) 193–198.  E. Dickinson, Hydrocolloids as emulsiﬁers and emulsion stabilizers, Food Hydrocoll. 23 (2009) 1473–1482.  B. Ozturk, S. Argin, M. Ozilgen, D.J. McClements, Formation and stabilization of nanoemulsion-based vitamin E delivery systems using natural surfactants: Quillaja saponin and lecithin, J. Food Eng. 142 (2014) 57–63.  Z.L. Wan, L.Y. Wang, J.M. Wang, Q. Zhou, Y. Yuan, X.Q. Yang, Synergistic interfacial properties of soy protein-stevioside mixtures: relationship to emulsion stability, Food Hydrocoll. 39 (2014) 127–135.  K. Muhammad, N.I.M. Zahari, S.P. Gannasin, N.M. Adzahan, J. Bakar, High methoxyl pectin from dragon fruit (Hylocereus polyrhizus) peel, Food Hydrocoll. 42 (2014) 289–297.  Committee on Chemicals Codex, Food chemical codex, National Academy of Sciences, Monograph Speciﬁcations–Pectin, Washington, D.C. 1996, pp. 283–286.  Y. Zouambia, K.Y. Ettoumi, M. Krea, N. Moulai-Mostefa, A new approach for pectin extraction: electromagnetic induction heating, Arab. J. Chem. 10 (4) (2014) 480–487.  N. Filisetti-Cozzi, N.C. Carpita, Measurement of uronic acids without interference from neutral sugars, J, Anal. Biochem. 197 (1) (1991) 157–162.  O.H. Lowry, N.J. Rosebrough, A.L. Farr, R.J. Randall, Protein measurement with the Folin phenol reagent, J. Biol. Chem. 193 (1) (1951) 265–275.  M. Wang, B. Huang, Ch. Fan, K. Zhao, H. Hu, X. Xu, S. Pan, F. Liu, Characterization and functional properties of mango peel pectin extracted by ultrasound assisted citric acid, Int. J. Biol. Macromol. 91 (2016) 794–803.  C.H. Tang, L. Shen, Dynamic adsorption and dilatational properties of BSA at oil/ water interface: role of conformational ﬂexibility, Food Hydrocoll. 43 (2015) 388–548.  F. Yuan, D. Xu, X. Qi, J. Zhao, Y. Gao, Impact of high hydrostatic pressure on the emulsifying properties of whey protein isolate–chitosan mixtures, Food Bioprocess Technol. 6 (2013) 1024–1031.  D. Xu, X. Wang, J. Jiang, F. Yuan, Y. Gao, Impact of whey protein–beet pectin conjugation on the physicochemical stability of β-carotene emulsions, Food Hydrocoll. 28 (2012) 258–266.  K. Alba, V. Kontogiorgos, Pectin at the oil-water interface: relationship of molecular composition and structure to functionality, Food Hydrocoll. 68 (2016) 211–218.  A.A. Perez, C. Carrera-Sánchez, J.M. Rodríguez-Patino, A.C. Rubiolo, L.G. Santiago, Surface adsorption behavior of milk whey protein and pectin mixtures under conditions of air-water interface saturation, Colloids Surf. B: Biointerfaces 85 (2011) 306–315.  M.J. Kim, H.K. Ju, Y. Kim, S.-H. Yoo, Y.-S. Kim, Eﬀects of amidation and/or methylesteriﬁcation of pectin on aroma release at diﬀerent calcium concentration, Food Hydrocoll. 52 (2016) 343–349.  Y. Zouambia, N. Moulai-Mostefa, K. Mohamed, Structural characterization and surface activity of hydrophobically functionalized extracted pectins, Carbohydr. Polym. 78 (2009) 841–846.  H.-m. Chen, X. Fu, Z.-g. Luo, Eﬀect of molecular structure on emulsifying properties of sugar beet pulp pectin, Food Hydrocoll. 54 (2016) 99–106.  L.C. Vriesmann, C.L.O. Petkowicz, Highly acetylated pectin from cacao pod husks